#------------------------------------------------------------------------------
#$Date: 2022-04-22 00:55:09 +0300 (Fri, 22 Apr 2022) $
#$Revision: 274623 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/12/99/7129999.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7129999
loop_
_publ_author_name
'Guo, Lixia'
'Han, Xue'
'Ma, Yujie'
'Li, Jiangnan'
'Lu, Wanpeng'
'Li, Weiyao'
'Lee, Daniel'
'da Silva, Ivan'
'Cheng, Yongqiang'
'Rudić, Svemir'
'Manuel, Pascal'
'Frogley, Mark D.'
'Ramirez-Cuesta, Anibal J.'
'Schröder, Martin'
'Yang, Sihai'
_publ_section_title
;
 High capacity ammonia adsorption in a robust metal--organic framework
 mediated by reversible host--guest interactions
;
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/D2CC01197B
_journal_year                    2022
_chemical_formula_sum            'C8 H4 O5 Sc'
_chemical_formula_weight         225.07
_chemical_name_mineral           ?MFM-300-Sc_empty?
_space_group_IT_number           98
_space_group_name_Hall           'I 4bw 2bw'
_space_group_name_H-M_alt        'I 41 2 2'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'I 41 2 2'
_audit_update_record
;
2022-01-17 deposited with the CCDC.	2022-04-11 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   15.3819(3)
_cell_length_b                   15.3819(3)
_cell_length_c                   12.4454(2)
_cell_measurement_temperature    7
_cell_volume                     2944.62(9)
_diffrn_ambient_temperature      7
_diffrn_measurement_device_type  neutron
_exptl_crystal_density_diffrn    1.082
_exptl_crystal_description       powder
_pd_proc_ls_prof_R_factor        1.42
_pd_proc_ls_prof_wR_expected     0.41
_pd_proc_ls_prof_wR_factor       1.54
_refine_ls_goodness_of_fit_all   3.77
_cod_data_source_file            d2cc01197b2.cif
_cod_data_source_block           1
_cod_original_cell_volume        2944.62(12)
_cod_original_sg_symbol_H-M      I4122
_cod_database_code               7129999
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 -y,1/2+x,1/4+z
3 1/2-x,1/2-y,1/2+z
4 1/2+y,-x,3/4+z
5 x,1/2-y,1/4-z
6 1/2+y,1/2+x,1/2-z
7 1/2-x,y,3/4-z
8 -y,-x,-z
9 1/2+x,1/2+y,1/2+z
10 1/2-y,x,3/4+z
11 -x,-y,z
12 y,1/2-x,1/4+z
13 1/2+x,-y,3/4-z
14 y,x,-z
15 -x,1/2+y,1/4-z
16 1/2-y,1/2-x,1/2-z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Sc Sc 8 0.68567(9) 0.31433(9) 0.5 1 1.77(6)
O1 O 8 0.7474(2) 0.25 0.625 1 0.50(5)
O2 O 16 0.6051(3) 0.3758(3) 0.6152(2) 1 0.50(5)
O3 O 16 0.5987(3) 0.2908(2) 0.7601(3) 1 0.50(5)
C1 C 16 0.5826(2) 0.36255(18) 0.71255(19) 1 0.82(4)
C2 C 16 0.53757(9) 0.43073(7) 0.77064(17) 1 0.82(4)
C3 C 8 0.5 0.5 0.7144(2) 1 0.82(4)
C4 C 16 0.53757(9) 0.43073(7) 0.88309(12) 1 0.82(4)
C5 C 8 0.5 0.5 0.93932(11) 1 0.82(4)
H1 H 8 0.8059(5) 0.25 0.625 1 0.50(5)
H3 H 8 0.5 0.5 0.6300(3) 1 0.82(4)
H4 H 16 0.56575(17) 0.37877(18) 0.92528(17) 1 0.82(4)
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Sc O2 88.46(11) . . . no
O1 Sc O1 97.23(9) . . 4_564 no
O1 Sc O3 84.64(13) . . 4_564 no
O1 Sc O3 88.23(13) . . 5_556 no
O1 Sc O2 172.49(12) . . 8_666 no
O1 Sc O2 172.49(12) 4_564 . . no
O2 Sc O3 97.21(17) . . 4_564 no
O2 Sc O3 90.66(17) . . 5_556 no
O2 Sc O2 86.32(15) . . 8_666 no
O1 Sc O3 88.23(13) 4_564 . 4_564 no
O1 Sc O3 84.64(13) 4_564 . 5_556 no
O1 Sc O2 88.46(11) 4_564 . 8_666 no
O3 Sc O3 169.22(17) 4_564 . 5_556 no
O2 Sc O3 90.66(17) 8_666 . 4_564 no
O2 Sc O3 97.21(17) 8_666 . 5_556 no
Sc O1 Sc 125.50(16) . . 2_645 no
Sc O2 C1 136.9(3) . . . no
Sc O3 C1 139.5(3) 2_645 . . no
Sc O1 H1 117.25(8) . . . no
Sc O1 H1 117.25(8) 2_645 . . no
O2 C1 O3 121.7(3) . . . no
O2 C1 C2 119.2(3) . . . no
O3 C1 C2 119.1(3) . . . no
C1 C2 C3 119.9(2) . . . no
C3 C2 C4 120.00(14) . . . no
C1 C2 C4 119.91(15) . . . no
C2 C3 C2 120.0(2) . . 11_665 no
C2 C4 C5 120.00(11) . . . no
C4 C5 C5 120.00(8) 11_665 . 8_667 no
C4 C5 C5 120.00(8) . . 8_667 no
C4 C5 C4 120.00(13) . . 11_665 no
C2 C3 H3 120.00(12) . . . no
C2 C3 H3 120.00(12) 11_665 . . no
C2 C4 H4 120.01(17) . . . no
C5 C4 H4 119.99(18) . . . no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sc O1 2.0739(17) . . no
Sc O2 2.118(4) . . no
Sc O1 2.0739(17) . 4_564 no
Sc O3 2.103(4) . 4_564 no
Sc O3 2.103(4) . 5_556 no
Sc O2 2.118(4) . 8_666 no
O2 C1 1.276(4) . . no
O3 C1 1.277(4) . . no
O1 H1 0.900(8) . . no
C1 C2 1.450(3) . . no
C2 C3 1.3997(19) . . no
C2 C4 1.400(3) . . no
C4 C5 1.3996(14) . . no
C5 C5 1.5104(19) . 8_667 no
C3 H3 1.050(4) . . no
C4 H4 1.050(3) . . no
